A simple planestrain solution for functionally graded multilayered isotropic cylinders


 Hillary Nash
 1 years ago
 Views:
Transcription
1 Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) A simple planestrain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The University of Akron, Akron, OH , USA A. K. Roy Air Force Research Laboratory, Materials and Manufacturing Directorate, AFRL/MLBC, 2941 P St., WPAFB, OH , USA (Received April 7, 2006, Accepted July 11, 2006) Abstract. A simple planestrain solution is derived in this paper for the functionally graded multilayered isotropic elastic cylinder under static deformation. The solution is obtained using method of separation of variables and is expressed in terms of the summation of the Fourier series in the circumferential direction. While the solution for order n = 0 corresponds to the axisymmetric deformation, that for n = 2 includes the special deformation frequently utilized in the upper and lower bounds analysis. umerical results for a threephase cylinder with a middle functionally graded layer are presented for both axisymmetric (n = 0) and general (n = 2) deformations, under either the traction or displacement boundary conditions on the surface of the layered cylinder. The solution to the general deformation case (n =2) is further utilized for the first time to find the upper and lower bounds of the effective shear modulus of the layered cylinder with a functionally graded middle layer. These results could be useful in the future study of cylindrical composites where FGMs and/or multilayers are involved. Keywords: elasticity; analytical solution; micromechanics; functionally graded material; fiber/matrix bond; effective modulus; threephase cylinder. 1. Introduction Functionally graded materials (FGMs) are continuously playing an important role in the design of composite structures. Besides their wellknown applications in thermal coatings for high temperature resistance, FGMs can be utilized as transition layers to reduce the sharp contrast of the material properties between the laminates (i.e., Zhu et al. 1996, Yang and Munz 1997). To assist the design of FGMs, various modeling and simulation methods have been proposed, including both numerical and analytical approaches (i.e., Aihara et al. 1998, Jin et al. 2002). While many analytical results have been reported so far, they are mostly associated with plate geometry only (i.e., Pan 2003, Zhong and Shang 2003, Pan and Feng 2005). To the best of the authors Associate Professor, Corresponding author,
2 2 E. Pan and A. K. Roy knowledge, the corresponding FGM cylindrical composite has not been fully investigated except for some simple deformation cases (Horgan and Chan 1999, Alshits et al. 2001, Oral and Anlas 2005). The present study was motivated by recent experimental work on fiber reinforced composites where it was observed that an FGM interface exists between the fiber and the matrix (Lafdi 2005). As such, from the fabrication and design points of view, it would be helpful if one could understand the effect of different FGMs on the distribution of the displacement, strain, and stress. The ability to estimate the effective material property is also an important issue in the corresponding FGM cylindrical composites. In this paper, we first present the general solution for the FGM cylinder layer by virtue of the method of separation of variables where the θdependent solution in the circumferential direction is expressed in terms of the Fourier series. For multilayered FGM cylinders, a system of linear equations are formed, which can be solved for the given boundary conditions. We discuss further in detail the cases which correspond to the axisymmetric deformation (n = 0) and the deformation of order n = 2 which has been frequently used in the upper and lower bounds analysis. We point out that our formulation for the upper and lower bounds of the shear modulus is presented based on a very simple approach associated with the strain energy and can be for both multilayered and FGM cases. As examples, numerical results on the displacement, strain, and stress are presented for the threephase cylinder with a FGM middle layer. The analysis shows clearly the influence of the FGM layer on the field distribution in the inner and outer homogeneous layers as well as in the FGM layer. The corresponding effective shear moduli for the threephase cylinder with FGM middle layer or with homogeneous middle layer are also predicted for the first time based on the solution. Results in this paper could be useful in future numerical study of the layered FGM cylindrical composites based on either boundary or finite element method. The paper is organized as follows: In Section 2, the general solution for the multilayered FGM cylinder is derived based on the method of separation of variables. In Section 3, the upper and lower bounds formulation is presented for the FGM and multilayered cylinder, which is based on the simple energy equivalence in the radical direction only. umerical examples are presented in Section 4 to show the influence of the FGM layer on displacement, strain, and stress fields as well as on the upper and lower bounds. Finally, conclusions are drawn in Section 5. Fig. 1 A threephase FGM composite cylinder
3 A simple planestrain solution for functionally graded multilayered isotropic cylinders 3 2. General solutions for the multilayered FGM cylinder Assume that a layered cylinder consists of L layers, which can be homogeneous or FGM (a threelayered cylinder is shown in Fig. 1). The layered cylinder is solid so that it includes the inner most layer (r = 0) j = 1. For any layer j of the cylinder bounded by r = R j 1, R j (R j > R j 1 ), we assume the Young s modulus as a function of radius in the form of E j r ( r ) E 0j  R where R is a nominal length within the layer j, k is the FGM factor which characterizes the variation of the Young s modulus within the layer, and E 0j is the proportional constant. To find the general solution for each layer, we utilize the method of separation of variables with Fourier series in the θdirection (as a summation from 0 to a large but finite ). In other words, we assume that the displacement, strain, and stress fields can be expressed as k (1) u r ε r ( r, θ ) ε rn ( r )e inθ ( r, θ ) u rn ( r )e inθ ; u θ ( r, θ ) i u θn ( r )e inθ ; ε θ ( r, θ ) ε θn ( r )e inθ ; γ rθ ( r, θ ) i γ rθn r σ r ( r, θ ) σ rn ( r )e inθ ; σ θ ( r, θ ) σ θn ( r )e inθ ; τ rθ ( r, θ ) i τ rθn r ( )e inθ ( )e inθ (2) (3) (4) where i = ( 1), and the shear stress τ rθ is also represented alternatively as σ rθ. We remark that while n = 0 corresponds to the axisymmetric deformation, n = 2 corresponds to the case used most frequently in the upper and lower bounds moduli estimation for threephase composites (i.e., Christensen and Lo 1979, Qiu and Weng 1991). It is emphasized, however, that the solution presented here is more general, which includes multilayered FGMs with the formulation being very simple. For example, in order to solve the general problem in the rθ space, it is sufficient for us to look at the corresponding amplitude of the field quantities for the given order n (or the rdependent function only). Keeping this in mind, the straindisplacement relations and the equilibrium equations in terms of the amplitudes are then reduced to (being functions of the variable r only) ε rn du rn /dr; ε θn u rn /r nu θn /r γ rθn nu rn /r du θn /dr u θn /r dσ rn /dr nτ rθn /r ( σ rn σ θn )/r 0 dτ rθn /dr nσ θn /r 2τ rθn /r 0 (5) (6) The constitutive relation between the stress and strain is similar to the wellknown Hooke s law with the exception that the Young s modulus is now a function of the radius r. Eqs. (5) and (6), combined with the isotropic constitutive relation, can be used to solve the unknown amplitudes of the displacement, strain, and stress fields. More specifically, in order to find
4 4 E. Pan and A. K. Roy the amplitude of the displacement field in each FGM layer, we assume the nth order solution as u rn ( r ) u θn ( r ) c 1 c 2 r p (7) where the unknown factor p and the corresponding coefficients (c 1 and c 2 ) can be solved from the following eigensystem of equations: { 2( k p 1) [( 1 ν j )p ν j ] n 2 ( 1 2ν j ) 21 ( 2ν j )( p 1 )}c 1 { 2ν j n( k p 1) n( 1 2ν j )( p 1) 2n( 1 2ν j )}c 2 0 { n( 1 2ν j )( k p 1 ) 2n( ν j p 1 ν j ) 2n( 1 2ν j )}c 1 {( 1 2ν j )( k p 1 )( p 1) 2n 2 ( 1 ν j ) 21 ( 2ν j )( p 1 )}c 2 0 (8) where ν j is the Poisson s ratio of the layer j, and k again characterizes the FGM as given in Eq. (1). For any layer other than the inner layer (r = 0), there are generally four different (complex) roots p m with four different (complex) pairs of eigenvectors (c 1m, c 2m ) (see Appendix A for detailed discussion). Therefore, the amplitudes of the displacements can be obtained as u rn ( r ) u θn ( r ) 4 c Re b 1m m r pm m 1 c 2m (9) where Re stands for the real part of the complex function. Once the displacement amplitudes are found, amplitudes of the strains are obtained using the displacementstrain relation, and stresses using the constitutive relation. It is obvious that for the solution to be bounded for the inner layer (r = 0), it is necessary to choose solutions corresponding to the two roots which have a positive real part. Once the general solution for each layer is derived, the boundary condition as well as the interface condition can be applied to solve all the unknowns involved in the layered cylinder (assuming continuity of the displacement and traction vectors at the interfaces between adjoining layers). The size of the system of linear equations will be proportional to the number of layers. Alternatively, it is possible to find the propagator matrix for each layer and then propagate the solutions from layer to layer (i.e., Pan 1997) to arrive at a system of equations involving only 2 unknowns. The propagator matrix (or transfer matrix) has been utilized previously in many areas including those related to laminate FGM composites (e.g., Pan 2001, 2003, Pan and Han 2005). In this paper, however, the direct solution method is adopted as the number of layers studied here is relatively small. 3. Upper and lower bounds of the effective shear modulus for multilayered FGM cylinders In this section, we follow the general procedure as in Christensen and Lo (1979) and Qiu and Weng (1991) for threephase composites in order to find both the upper and lower bounds of the effective shear modulus for multilayered FGM cylinders. It can be observed that the formulation
5 A simple planestrain solution for functionally graded multilayered isotropic cylinders 5 presented here is extremely simple with all the calculations in the radial rdirection only. In order to obtain the upper bound, we apply the following displacement condition on the surface of the outer layer r = R L (in terms of the Cartesian coordinates (x 1, x 2 ) in the (r, θ )plane): u α ( r R L ;θ ) ε αβ x β (10) where the described nonzero components of the strain tensor are ε 11 ε 22 ε (11) It is easy to show that in terms of the polar coordinates, the displacement boundary condition becomes u r ( r R L ;θ ) u θ ( r R L ;θ ) ε R L cos2θ sin2θ (12) Or in general, u r ( r R L ;θ ) u θ ( r R L ;θ ) ε R L e 2iθ ie 2iθ (13) Therefore, the displacement amplitudes of second order (n = 2) should satisfy the following boundary condition: u r2 ( r R L ) ε R L (14) u θ2 ( r R L ) Again, the subscript 2 on the lefthand side of the equation indicates the amplitude of the displacement corresponding to order n = 2. Similarly, to find the lower bound, the traction boundary condition on the surface of the outer layer r = R L (again, in terms of the Cartesian coordinates) is described by: t α ( r R L ;θ ) σ αβ n β (15) where the described nonzero components of the stress tensor are σ 11 σ 22 σ (16) In terms of the polar coordinates, the traction boundary condition becomes σ r ( r R L ;θ ) τ rθ ( r R L ;θ ) σ cos2θ sin2θ (17) Or in general, σ r ( r R L ;θ ) τ rθ ( r R L ;θ ) σ e2iθ ie 2iθ (18)
6 6 E. Pan and A. K. Roy Therefore, the corresponding traction amplitudes of order n = 2 satisfy the following boundary condition: σ r2 ( r R L ) τ rθ2 ( r R L ) σ (19) In both cases, the effective shear modulus G eff is calculated based on the equivalence of the strain energies between the multilayered FGM model and the homogeneous model with the effective shear modulus. The derivation is presented below: Since both the multilayered FGM and the homogeneous models have the same θdependence, multiple factors from integration over the variable θ are therefore the same on both sides of the energy equation. Consequently, it is only necessary to carry out the integration along the radial direction. For a linear elastic cylinder made of L FGM layers, the strain energy is calculated from L 1 R E Total j  σ αβ2 ( r )ε αβ2 ( r )rdr 2 R j 1 j L j 1 R j R j 1 2G ν 1 2ν [( )( ε r2 ε θ2 ) 2νε r2 ε θ2 ] Gγ rθ2 rdr (20) This expression can be used to find energy in the multilayered FGM model once all the coefficients in each layer are solved under the given boundary and interface conditions. The energy for the corresponding homogeneous model with the undetermined effective shear modulus G eff is evaluated based on simple surface integration where the θ integration cancels out when equating this expression to that of the multilayered FGM model in Eq. (20). For the equivalent homogeneous model, the total energy is E 1  σ αβ2 ε αβ2 dv σ αβ2 n β u α2 ds 2 Ignoring the θdependent factor, the effective energy is therefore reduced to (21) 1 E eff  σ αβ2 n β u α2 R L (22) 2 Using either the displacement or traction boundary condition, combined with the solved coefficients for the equivalent model, it can be shown that the expression for the effective energy Eq. (22) involves only the effective shear modulus as the unknown. Letting the effective energy Eq. (22) equal the multilayered FGM energy Eq. (20), then the effective shear modulus G eff can be finally solved. 4. umerical examples 4.1 Example 1: Upper and lower bounds of shear modulus in threephase cylinders We first checked our solution of multilayered cylinders for the effective shear modulus. For the
7 A simple planestrain solution for functionally graded multilayered isotropic cylinders 7 Fig. 2 Comparison of the amplitudes (n = 2) of stresses based on the FGM vs. discrete layered models under the displacement boundary condition Table 1 Upper and lower bounds of the effective shear modulus G eff for the threephase composite with ν 1 = ν 2 = ν 3 =0.3 and d 2 :d 1 =2:1 E 1 /E 2 /E 3 Fraction d 1 Upper G eff Lower G eff 1/5/25 25/5/1 25/1/ threephase cylinder case considered in Qiu and Weng (1991), the Young s modulus E i in each layer takes a value of 1, 5, or 25 (for example, E 1 /E 2 /E 3 = 1/5/25 for one of the models), whilst the Poisson s ratio is the same, i.e., ν 1 = ν 2 = ν 3 = 0.3. The upper and lower bounds for the shear modulus predicted from our analytical formulation are found to be the same as those in Qiu and Weng (1991, Figs. 1 and 2). For instance, listed in Table 1 are some of the results from our solution for different volumetric fractions d 1 (with fixed d 2 :d 1 = 2:1). The corresponding radii of the threephase cylinder are given in Table 2.
8 8 E. Pan and A. K. Roy Table 2 Volumetric fraction d 1 and the corresponding radii of the threephase cylinder for fixed ratio d 2 :d 1 =2:1 d 1 R 1 R 2 R Example 2: A threephase cylinder with a middle FGM layer (n = 2) The second example is for a threephase cylinder with a middle FGM layer. Solutions for both the direct FGM and discrete models are employed to carry out the calculation. In the discrete model, a total of 12 layers are used. In other words, 10 discrete homogeneous layers are used to approximate the middle FGM layer (it has been checked that when the number of the discrete layers is equal to 10 or larger, the discretebased solution is nearly the same as the FGM solution). The FGM factor k in Eq. (1) is chosen in such a way that E 2 (r) = (r/r 1 ) in the FGM layer. Other parameters are R 1 = 1.0, R 2 = 2.0, and R 3 = 3.0, ν 1 = ν 2 = ν 3 = 0.3, E 1 = 1 and E 3 = 25. It is obvious that when r = R 1 we have E 2 = 1, and at r = R 2, we have E 2 = 5. The boundary condition applied at R 3 = 3.0 is the displacement condition described by Eq. (14) with ε 1. For example, the amplitudes of the stresses from both the direct FGM and discrete homogeneous models are plotted in Fig. 2. It is observed that both models predict very close results to each other. Furthermore, there is a sharp discontinuity for the normal stress σ θ across the interface at r = 2 due to the jump of the Young s moduli on both sides of the interface. We have also compared this FGM model to a couple of discrete homogeneous threephase models with different combinations of E 1 /E 2 /E 3. While the results for the upper and lower bounds are given in Table 3, the amplitudes of the stress components for different models are presented in Figs. 3(a), 3(b), and 3(c) for the traction boundary condition Eq. (19) with σ 1. It is interesting to note from Table 3 that the shear modulus bounds for the FGM case is somewhere between those of the discrete models E 1 /E 2 /E 3 = 1/2/25 and E 1 /E 2 /E 3 = 1/3/25. From Fig. 3, we first observe that while the normal (σ r ) and shear (τ rθ ) stresses have approximately the same magnitude, the amplitude of the hoop stress σ θ is much larger. For different combinations of E 1 /E 2 /E 3, the stress amplitude could decrease in one layer and increase in another for increasing E 2 in the middle layer. For instance, with increasing E 2, the amplitude of σ r decreases in layers 1 and 2 but increases in layer 3 (Fig. 3(a)). However, the trend for the FGM layer case is different: while the stress variation for the FGM layer model follows the curve of one of the discrete models E 1 /E 2 /E 3 in layers 1 and 3, its behavior in the FGM middle layer is different: It Table 3 Upper and lower bounds of the shear modulus for the FGM middle layer model and the discrete homogeneous models with different combinations of E 1 /E 2 /E 3 E 1 /E 2 /E 3 Upper G eff Lower G eff 1/2/ FGM /3/ /5/
9 A simple planestrain solution for functionally graded multilayered isotropic cylinders 9 Fig. 3 Amplitudes (n = 2) of stresses in FGM and discrete layered cylinders under traction boundary condition: Stress σ r in (a), σ θ in (b), and σ rθ in (c) crosses some (Figs. 3(a) and 3(c)) or all (Fig. 3(b)) of the curves predicted based on the discrete models E 1 /E 2 /E 3 in the middle layer. More importantly, the stress variation in the FGM middle layer is much smoother than those in the homogeneous middle layer, and there is no discontinuity for the stress σ θ across the interface between the FGM and the inner layer as the Young s moduli is continuous there. 4.3 Example 3: A threephase cylinder with a middle FGM layer (n = 0) The effect of different k values in the FGM model (Eq. (1)) is studied in this example, where the
10 10 E. Pan and A. K. Roy Fig. 4 Young s modulus in the middle FGM layer of a threephase cylinder k in the middle FGM layer (1 < r <2) varies as k = 0, 1/2, 1, 2, 3, 4, 5. The deformation is restricted to the axisymmetric case (i.e., n = 0) under uniform traction (i.e., σ r0 (( r R 3 ) 1). While the Poisson s ratios are the same in the three layers (i.e., ν 1 = ν 2 = ν 3 = 0.3), the Young s moduli in the inner layer (r < 1) and outer layer (2 < r < 5) are, respectively, E 1 = 10 and E 3 = 1. The Young s modulus E 2 in the FGM middle layer (1 < r < 2) is described by Eq. (1) with E 02 = 10 and its distribution for different k is plotted in Fig. 4. The corresponding solutions for the displacement, strain, and stress are presented in Figs. 5(a), 5(b), and 5(c). Some interesting features can be observed from Fig. 5: 1) Since the Young s modulus in the inner layer is larger than those in the other two layers, the induced displacement and strain fields in this layer are much smaller. Therefore, the effect of different k values on the displacement and strain fields within layer 1 (r < 1) cannot be clearly observed (Figs. 5(a) and 5(b)). 2) For displacement u r (Fig. 5(a)), its values in both the FGM and outer layers increase with increasing magnitude of k. For strain ε r (Fig. 5(b)), however, with increasing magnitude of k, its value increases in the FGM layer, but decreases in the outer layer. 3) As for the stress in the inner layer, increasing magnitude of k corresponds to an increase of the stress value for k = 0 to 3; however, when k = 4 and 5, the stress amplitude is reduced, with the result for k = 5 close to that for k = 1/2 (Fig. 5(c)). This feature is possibly due to the fact that for k = 0 to 3, the Young s moduli in the FGM layer are all larger than that in the outer layer; however, for k = 4 and 5, they become smaller in the FGM layer than that in the outer layer (near r = 2 in the FGM layer in Fig. 4). 4) In the outer layer, the stress σ r decreases with increasing magnitude of k (Fig. 5(c)). In general, different k values have apparent effect on the displacement, strain, and stress in both the FGM middle layer and the outer layer. While the response (displacement, strain, or stress) as a
11 A simple planestrain solution for functionally graded multilayered isotropic cylinders 11 Fig. 5 Amplitudes (n = 0) of the field quantities for different FGM factors k: Radial displacement u r in (a), strain ε r in (b), stress σ r in (c) function of r is gentle in the outer layer, the one in the FGM layer experiences a large change in its amplitude. It is also obvious that, the transfer of the stress from the inner to the outer layer is more complicated than that of the displacement or strain, with the inner fiber carrying most of the stress. 5. Conclusions In this paper, exact solutions are derived for multilayered FGM cylinders under static deformation. They are obtained based on the method of separation of variables and include the previous
12 12 E. Pan and A. K. Roy axisymmetric solution as a special case. The most commonly used upper and lower bounds formulation is also extended to the general multilayered FGM case and is further presented in terms of a simple energy relation. While our solutions can be applied to many different deformation cases, illustrative results for a threephase cylinder with a FGM middle layer are presented for orders n = 0 and 2. It is observed clearly that the FGM middle layer can strongly influence the field (displacement, strain, and stress) distribution within the FGM layer and in the inner and outer layers as well. The FGM layer also has an obvious effect on the upper and lower bounds of the effective shear modulus. Results presented in this paper could be useful in future numerical analysis of FGM layered cylinders based on the boundary and finite element methods. Acknowledgements This work was carried out while the first author was at AFRL under the Air Force 2005 Summer Faculty Fellowship Program. References Aihara, T. Jr., Sho, T. and Kawazoe, Y. (1998), Molecular dynamics simulation on elastic behavior of i/i 3 Al interface with graded structure, J. Japan Institute of Metals, 62, Alshits, V.I. and Kirchner, H.O.K. (2001), Cylindrically anisotropic, radially inhomogeneous elastic materials, Proc. R. Soc. Lond, A 457, Christensen, R.M. and Lo, K.H. (1979), Solutions for effective shear properties in three phase sphere and cylinder models, J. Mech. Phys. Solids, 27, Horgan, C.O. and Chan, A.M. (1999), The pressurized hollow cylinder or disk problem for functionally graded isotropic linearly elastic materials, J. Elasticity, 55, Jin, Z.H., Paulino, G.H. and Dodds, Jr. R.H. (2002), Finite element investigation of quasistatic crack growth in functionally graded materials using a novel cohesive zone fracture model, J. Appl. Mech., 69, Lafdi, K. (2005), TEM characterization of the interface property between the fibre and matrix, Private Communication. Oral, A. and Anals, G. (2005), Effects of radially varying moduli on stress distribution of nonhomogeneous anisotropic cylindrical bodies, Int. J. Solids Struct., 42, Pan, E. (1997), Static Green s functions in multilayered halfspaces, Applied Mathematical Modelling, 21, Pan, E. (2001), Exact solution for simply supported and multilayered magnetoelectroelastic plates, ASME, J. Appl. Mech., 68, Pan, E. (2003), Exact solution for functionally graded anisotropic elastic composite laminates, J. Composite Mater., 37, Pan, E. and Han, F. (2005), Exact solution for functionally graded and layered magnetoelectroelastic plates, Int. J. Eng. Sci., 43, Qiu, Y.P. and Weng, G.J. (1991), Elastic moduli of thickly coated particle and fiberreinforced composites, J. Appl. Mech., 58, Tarn, J.Q. (2001), Exact solutions for functionally graded anisotropic cylinders subjected to thermal and mechanical loads, Int. J. Solids Struct., 38, Yang, Y.Y. and Munz, D. (1997), Reduction of residual stresses in a two dissimilar materials joint by using a functionally graded material, In Composites and Functionally Graded Materials, Proc. of the Symposia, ASME International Mechanical Engineering Congress and Exposition, Dallas, TX, Zhong, Z. and Shang, E.T. (2003), Threedimensional exact analysis of a simple supported functionally gradient
13 A simple planestrain solution for functionally graded multilayered isotropic cylinders 13 piezoelectric plate, Int. J. Solids Struct., 40, Zhu, J., Yin, Z., Mao, J., Lai, Z., Yang, D., ing, X. and Li, D. (1996), Interface structure of ZrO 2 i functionally gradient material, Acta Metallurgica Sinica, 32, Appendix A: Roots of the eigensystem of Eqs. (8) Using Mathematica, the four different roots p m (m = 1, 2, 3, 4) of the system of Eq. (8) can be found as (for simplicity, the Poisson s ratio in layer j, ν j, has been replaced with ν ): where p 1 4 k ± k a± b ( ν) (A1) a 1 2n 2 ( 1 ν ) 1 k ( )( 1 2ν ) b k 2 16n 2 2 ( 1 ν ) 8n 2 ( k 4ν) 8kn 2 ν( 3 2ν) 4k 2 n 2 ν 1 ν ( ) (A2) We remark that in general the four roots are complex. Therefore, the corresponding eigenvectors (c 1m, c 2m ) are also complex. Since the displacement solution is real, one needs to take only the real part of the complex solution. We discuss below the solutions corresponding to those with special functional gradient k and Poisson s ratio v values: 1) k = 0 This corresponds to the homogeneous material case. For this case, the four roots p m in Eq. (A1) are real, and can be expressed as n± 1 p 1 4 ±( ) (A3) The same roots can also be easily derived from the governing equations when the material is homogeneous. 2) n = 0 This corresponds to the axisymmetric deformation studied in detail in the paper. For the axisymmetric case, the four roots p m are k/2± k 2 /4 k 1; m 1, 2 p m k/2± k 2 /4 k kν/ ( 1 ν ); m 3, 4 It is obvious that for the regular domain of k 0 and 0 ν 1/2, all the roots in Eq. (A4) are real. (A4) 3) n =2 This corresponds to the special deformation associated with the prediction of the effective shear modulus, as discussed in the paper. For this case, a 10( 1 ν ) k 1 2ν b k 2 2 ( 1 16ν 16ν ) 32k 1 2ν ( ) ( ) 1 ν ( ) 64 1 ν ( ) 2 (A5) It is apparent that for n = 2 and also for other orders, the four roots will be, in general, complex (in pair). For example, for ν = 0.3, the four roots are
14 14 E. Pan and A. K. Roy k ± 1.96k k ± k 2.36k 2 p 1 4 ( ) (A6) which, for the special functional gradient k = 3 studied in the paper, become ± i; m 1, 2 p m ± i; m 3, 4 (A7)
Module 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationStresses and Displacements in Functionally Graded Materials of SemiInfinite Extent Induced by Rectangular Loadings
Materials 2012, 5, 210226; doi:10.3390/ma5020210 Article OPEN ACCESS materials ISSN 19961944 www.mdpi.com/journal/materials Stresses and Displacements in Functionally Graded Materials of SemiInfinite
More information17th European Conference on Fracture 25 September,2008, Brno, Czech Republic. Thermal Fracture of a FGM/Homogeneous Bimaterial with Defects
5 September,8, Brno, Czech Republic Thermal Fracture of a FGM/Homogeneous Bimaterial with Defects Vera Petrova, a, Siegfried Schmauder,b Voronezh State University, University Sq., Voronezh 3946, Russia
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationInhomogeneity Material Effect on Electromechanical Stresses, Displacement and Electric Potential in FGM Piezoelectric Hollow Rotating Disk
Journal of Solid Mechanics Vol. 2, No. 2 (2010) pp. 144155 Inhomogeneity Material Effect on Electromechanical Stresses, Displacement and Electric Potential in FGM Piezoelectric Hollow Rotating Disk A.
More informationfunctionally graded material, piezoelectric material, circular plates, uniform electric potential, direct displacement
Science in China Series G: Physics, Mechanics & Astronomy 008 SCIENCE IN CHINA PRESS SpringerVerlag www.scichina.com phys.scichina.com www.springerlink.com Threedimensional analytical solution for a
More informationU.S. South America Workshop. Mechanics and Advanced Materials Research and Education. Rio de Janeiro, Brazil. August 2 6, Steven L.
Computational Modeling of Composite and Functionally Graded Materials U.S. South America Workshop Mechanics and Advanced Materials Research and Education Rio de Janeiro, Brazil August 2 6, 2002 Steven
More informationGraduate School of Engineering, Kyoto University, Kyoto daigakukatsura, Nishikyoku, Kyoto, Japan.
On relationship between contact surface rigidity and harmonic generation behavior in composite materials with mechanical nonlinearity at fibermatrix interface (Singapore November 2017) N. Matsuda, K.
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationScienceDirect. Hamiltonian approach to piezoelectric fracture
Available online at www.sciencedirect.com ScienceDirect Procedia Materials Science 3 ( 014 ) 318 34 0th European Conference on Fracture (ECF0) Hamiltonian approach to piezoelectric fracture J.M. Nianga
More informationSemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials
International Journal of Composite Materials 2017, 7(3): 103114 DOI: 10.5923/j.cmaterials.20170703.03 SemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju
More informationCRACK INITIATION CRITERIA FOR SINGULAR STRESS CONCENTRATIONS Part I: A Universal Assessment of Singular Stress Concentrations
Engineering MECHANICS, Vol. 14, 2007, No. 6, p. 399 408 399 CRACK INITIATION CRITERIA FOR SINGULAR STRESS CONCENTRATIONS Part I: A Universal Assessment of Singular Stress Concentrations Zdeněk Knésl, Jan
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationTwodimensional ternary locally resonant phononic crystals with a comblike coating
Twodimensional ternary locally resonant phononic crystals with a comblike coating YanFeng Wang, YueSheng Wang,*, and Litian Wang Institute of Engineering Mechanics, Beijing Jiaotong University, Beijing,
More informationSettlement analysis of viscoelastic foundation under vertical line load using a fractional KelvinVoigt model
Geomechanics and Engineering, Vol. 4, No. 1 (01) 6778 67 Technical Note Settlement analysis of viscoelastic foundation under vertical line load using a fractional KelvinVoigt model HongHu Zhu* 1, LinChao
More informationCurvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment. P. Krulevitch G. C. Johnson
UCRLJC30440 PREPRINT Curvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment P. Krulevitch G. C. Johnson This paper was prepared for submittal to the Materials Research Society Spring
More informationElements of Rock Mechanics
Elements of Rock Mechanics Stress and strain Creep Constitutive equation Hooke's law Empirical relations Effects of porosity and fluids Anelasticity and viscoelasticity Reading: Shearer, 3 Stress Consider
More informationSymmetric Bending of Beams
Symmetric Bending of Beams beam is any long structural member on which loads act perpendicular to the longitudinal axis. Learning objectives Understand the theory, its limitations and its applications
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationElements of Continuum Elasticity. David M. Parks Mechanics and Materials II February 25, 2004
Elements of Continuum Elasticity David M. Parks Mechanics and Materials II 2.002 February 25, 2004 Solid Mechanics in 3 Dimensions: stress/equilibrium, strain/displacement, and intro to linear elastic
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationA Piezoelectric Screw Dislocation Interacting with an Elliptical Piezoelectric Inhomogeneity Containing a Confocal Elliptical Rigid Core
Commun. Theor. Phys. 56 774 778 Vol. 56, No. 4, October 5, A Piezoelectric Screw Dislocation Interacting with an Elliptical Piezoelectric Inhomogeneity Containing a Confocal Elliptical Rigid Core JIANG
More informationAnalysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method
Analysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method V.M.F. Nascimento Departameto de ngenharia Mecânica TM, UFF, Rio de Janeiro
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationCrack Tip Plastic Zone under Mode I Loading and the Nonsingular T zz stress
Crack Tip Plastic Zone under Mode Loading and the Nonsingular T stress Yu.G. Matvienko Mechanical Engineering Research nstitute of the Russian Academy of Sciences Email: ygmatvienko@gmail.com Abstract:
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationBack Analysis of Measured Displacements of Tunnels
Rock Mechanics and Rock Engineering 16, 173180 (1983) Rock Mechanics and Rock Engineering 9 by SpringerVerlag 1983 Back Analysis of Measured Displacements of Tunnels By S. Sakurai and K. Takeuchi Kobe
More informationBasic concepts to start Mechanics of Materials
Basic concepts to start Mechanics of Materials Georges Cailletaud Centre des Matériaux Ecole des Mines de Paris/CNRS Notations Notations (maths) (1/2) A vector v (element of a vectorial space) can be seen
More informationElastic plastic bending of stepped annular plates
Applications of Mathematics and Computer Engineering Elastic plastic bending of stepped annular plates JAAN LELLEP University of Tartu Institute of Mathematics J. Liivi Street, 549 Tartu ESTONIA jaan.lellep@ut.ee
More informationPEAT SEISMOLOGY Lecture 3: The elastic wave equation
PEAT8002  SEISMOLOGY Lecture 3: The elastic wave equation Nick Rawlinson Research School of Earth Sciences Australian National University Equation of motion The equation of motion can be derived by considering
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More informationAn alternative design method for the doublelayer combined die using autofrettage theory
https://doi.org/10.5194/ms82672017 Author(s) 2017. This work is distributed under the Creative Commons Attribution.0 License. An alternative design method for the doublelayer combined die using autofrettage
More informationTheoretical investigation on the fatigue life of elastomers incorporating material inhomogeneities
Theoretical investigation on the fatigue life of elastomers incorporating material inhomogeneities A. Andriyana Laboratoire Matériaux, Endommagement, Fiabilité et Ingénierie des Procédés LAMEFIP) École
More informationGeometrydependent MITC method for a 2node isobeam element
Structural Engineering and Mechanics, Vol. 9, No. (8) 33 Geometrydependent MITC method for a node isobeam element PhillSeung Lee Samsung Heavy Industries, Seocho, Seoul 37857, Korea HyuChun Noh
More informationModeling of Interphases in FiberReinforced Composites Under Transverse Loading Using the Boundary Element Method
Y. J. Liu 1 Assistant Professor, email: Yijun.Liu@uc.edu Mem. ASME N. Xu Graduate Student Department of Mechanical, Industrial, and Nuclear Engineering, P.O. Box 210072, University of Cincinnati, Cincinnati,
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationAxisymmetric Stress Analysis of Internally Pressurized Rotating Cylinder using Finite Element Method
Axisymmetric Stress Analysis of Internally Pressurized Rotating Cylinder using Finite Element Method A Project Report Submitted in partial fulfillment for the award of the degree Of BACHELOR OF TECHNOLOGY
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More informationFinite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure
Vibrations in Physical Systems Vol.26 (2014) Finite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure Abstract Maria NIENARTOWICZ Institute of Applied Mechanics,
More informationComputation of MixedMode Stress Intensity Factors for Cracks in ThreeDimensional Functionally Graded Solids
Computation of MixedMode Stress Intensity Factors for Cracks in ThreeDimensional Functionally Graded Solids Matthew C. Walters 1 ; Glaucio H. Paulino 2 ; and Robert H. Dodds Jr. 3 Abstract: This work
More informationInterfacial partial debonding and its in uence on the elasticity of a twophase composite
Mechanics of Materials 32 (2000) 695±709 www.elsevier.com/locate/mechmat Interfacial partial debonding and its in uence on the elasticity of a twophase composite S.F. Zheng, M. Denda, G.J. Weng * Department
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationFREE VIBRATION OF THERMALLY PRE/POSTBUCKLED CIRCULAR THIN PLATES EMBEDDED WITH SHAPE MEMORY ALLOY FIBERS
Journal of Thermal Stresses, 33: 79 96, 2010 Copyright Taylor & Francis Group, LLC ISSN: 01495739 print/1521074x online DOI: 10.1080/01495730903409235 FREE VIBRATION OF THERMALLY PRE/POSTBUCKLED CIRCULAR
More informationStresses in Curved Beam
Stresses in Curved Beam Consider a curved beam subjected to bending moment M b as shown in the figure. The distribution of stress in curved flexural member is determined by using the following assumptions:
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationReference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity",
Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity", Oxford University Press, Oxford. J. Lubliner, "Plasticity
More informationTransactions on Engineering Sciences vol 13, 1996 WIT Press, ISSN
Computational debonding analysis of a thermally stressed fiber/matrix composite cylinder F.G. Buchholz," O. Koca* "Institute ofapplied Mechanics, University ofpaderborn, D33098 Paderborn, Germany ^Institute
More informationThe Study of Thermal Stresses of a Two Phase FGM Hollow Sphere
Copyright 2015 Tech Science Press CMES, vol.109110, no.6, pp.537554, 2015 The Study of Thermal Stresses of a Two Phase FGM Hollow Sphere Baoyu Ma 1, Guansuo Dui 1, Shengyou Yang 2 and Libiao Xin 1 Abstract:
More informationThermoMechanical Response of Functionally Graded Materials for Extreme Environments
ThermoMechanical Response of Functionally Graded Materials for Extreme Environments Introduction In recent years, functionally graded materials (FGMs) have attracted much interest in a wide range of engineering
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationModeling and analysis of the electromechanical behavior of surfacebonded piezoelectric actuators using finite element method
Modeling and analysis of the electromechanical behavior of surfacebonded piezoelectric actuators using finite element method Huangchao Yu and Xiaodong Wang Abstract Piezoelectric actuators have been widely
More informationChapter 5 Torsion STRUCTURAL MECHANICS: CE203. Notes are based on Mechanics of Materials: by R. C. Hibbeler, 7th Edition, Pearson
STRUCTURAL MECHANICS: CE203 Chapter 5 Torsion Notes are based on Mechanics of Materials: by R. C. Hibbeler, 7th Edition, Pearson Dr B. Achour & Dr Eng. K. Elkashif Civil Engineering Department, University
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationLimit analysis of FGM circular plates subjected to arbitrary rotational symmetric loads using vonmises yield criterion
Acta Mech DOI 10.1007/s007070130828z M. Baghani B. Fereidoonnezhad Limit analysis of FGM circular plates subjected to arbitrary rotational symmetric loads using vonmises yield criterion Received: 7
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationLecture 3: The Concept of Stress, Generalized Stresses and Equilibrium
Lecture 3: The Concept of Stress, Generalized Stresses and Equilibrium 3.1 Stress Tensor We start with the presentation of simple concepts in one and two dimensions before introducing a general concept
More informationContinuum mechanics V. Constitutive equations. 1. Constitutive equation: definition and basic axioms
Continuum mechanics office Math 0.107 ales.janka@unifr.ch http://perso.unifr.ch/ales.janka/mechanics Mars 16, 2011, Université de Fribourg 1. Constitutive equation: definition and basic axioms Constitutive
More informationModified MaxwellGarnett equation for the effective transport coefficients in inhomogeneous media
J. Phys. A: Math. Gen. 3 (998) 7227 7234. Printed in the UK PII: S03054470(98)939762 Modified MaxwellGarnett equation for the effective transport coefficients in inhomogeneous media Juris Robert Kalnin
More informationVORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS
The 4 th World Conference on Earthquake Engineering October 7, 008, Beijing, China VORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS K.
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationA FAILURE CRITERION FOR POLYMERS AND SOFT BIOLOGICAL MATERIALS
Material Technology A FALURE CRTERON FOR POLYMERS AND SOFT BOLOGCAL MATERALS Authors: William W. Feng John O. Hallquist Livermore Software Technology Corp. 7374 Las Positas Road Livermore, CA 94550 USA
More informationPlane and axisymmetric models in Mentat & MARC. Tutorial with some Background
Plane and axisymmetric models in Mentat & MARC Tutorial with some Background Eindhoven University of Technology Department of Mechanical Engineering Piet J.G. Schreurs Lambèrt C.A. van Breemen March 6,
More informationDebonding process in composites using BEM
Boundary Elements XXVII 331 Debonding process in composites using BEM P. Prochazka & M. Valek Czech Technical University, Prague, Czech Republic Abstract The paper deals with the debonding fibermatrix
More informationDetermination of Poisson s Ratio of Rock Material by Changing Axial Stress and Unloading Lateral Stress Test
Rock Mech Rock Eng DOI 10.1007/s0060301405869 TECHNICAL NOTE Determination of Poisson s Ratio of Rock Material by Changing Axial Stress and Unloading Lateral Stress Test Xiangtao Xu Runqiu Huang Hua
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationSchur decomposition in the scaled boundary finite element method in elastostatics
IOP Conference Series: Materials Science and Engineering Schur decomposition in the scaled boundary finite element method in elastostatics o cite this article: M Li et al 010 IOP Conf. Ser.: Mater. Sci.
More informationAspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites
Aspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a
More informationExam paper: Biomechanics
Exam paper: Biomechanics Tuesday August 10th 2010; 9.0012.00 AM Code: 8W020 Biomedical Engineering Department, Eindhoven University of Technology The exam comprises 10 problems. Every problem has a maximum
More informationBasic Concepts of Strain and Tilt. Evelyn Roeloffs, USGS June 2008
Basic Concepts of Strain and Tilt Evelyn Roeloffs, USGS June 2008 1 Coordinates Righthanded coordinate system, with positions along the three axes specified by x,y,z. x,y will usually be horizontal, and
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationLocalization in Undrained Deformation
Localization in Undrained Deformation J. W. Rudnicki Dept. of Civil and Env. Engn. and Dept. of Mech. Engn. Northwestern University Evanston, IL 621319 John.Rudnicki@gmail.com Fourth Biot Conference on
More informationChapter 2. Rubber Elasticity:
Chapter. Rubber Elasticity: The mechanical behavior of a rubber band, at first glance, might appear to be Hookean in that strain is close to 100% recoverable. However, the stress strain curve for a rubber
More informationPredicting Elastic Properties of Unidirectional SU8/ZnO Nanocomposites using COMSOL Multiphysics
Predicting Elastic Properties of Unidirectional SU8/ZnO Nanocomposites using COMSOL Multiphysics Neelam Mishra 1, and Kaushik Das *1 1 School of Minerals Metallurgical and Materials Engineering, Indian
More informationModeling Contact between Rigid Sphere and Elastic Layer Bonded to Rigid Substrate
IEEE TRANSACTIONS ON COMPONENTS AND PACKAGING TECHNOLOGIES, VOL. 24, NO. 2, JUNE 2001 207 Modeling Contact between Rigid Sphere and Elastic Layer Bonded to Rigid Substrate Mirko Stevanović, M. Michael
More informationCRACKTIP DRIVING FORCE The model evaluates the eect of inhomogeneities by nding the dierence between the Jintegral on two contours  one close to th
ICF 100244OR Inhomogeneity eects on crack growth N. K. Simha 1,F.D.Fischer 2 &O.Kolednik 3 1 Department ofmechanical Engineering, University of Miami, P.O. Box 248294, Coral Gables, FL 331240624, USA
More informationEffects of a pulsed electromagnetic field on the impact response of electrically conductive. composite plates
Effects of a pulsed electromagnetic field on the impact response of electrically conductive composite plates 1. Introduction Electromagnetic solids encompass a broad class of materials in which the interaction
More information1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor.
Elasticity Homework Problems 2014 Section 1. The Strain Tensor. 1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor. 2. Given a steel bar compressed with a deformation
More informationAPPLICATION OF ISOTENSOIDBASED CROSS SECTIONS TO FILAMENTWOUND TOROIDAL PRESSURE VESSELS
APPLICATION OF ISOTENSOIDBASED CROSS SECTIONS TO FILAMENTWOUND TOROIDAL PRESSURE VESSELS L. Zu, S. Koussios and A. Beukers Design and Production of Composite Structures, Faculty of Aerospace Engineering
More informationA multiscale approach for composite materials as multifield continua
Materials Science Forum Vols. 539543 (27) pp. 25512556 online at http://www.scientific.net (27) Trans Tech Publications, Switzerland A multiscale approach for composite materials as multifield continua
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationMassachusetts Institute of Technology 22.68J/2.64J Superconducting Magnets. February 27, Lecture #4 Magnetic Forces and Stresses
Massachusetts Institute of Technology.68J/.64J Superconducting Magnets February 7, 003 Lecture #4 Magnetic Forces and Stresses 1 Forces For a solenoid, energy stored in the magnetic field acts equivalent
More informationSIMULATION OF PLANE STRAIN FIBER COMPOSITE PLATES IN BENDING THROUGH A BEM/ACA/HM FORMULATION
8 th GRACM International Congress on Computational Mechanics Volos, 12 July 15 July 2015 SIMULATION OF PLANE STRAIN FIBER COMPOSITE PLATES IN BENDING THROUGH A BEM/ACA/HM FORMULATION Theodore V. Gortsas
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationShear stresses around circular cylindrical openings
Shear stresses around circular cylindrical openings P.C.J. Hoogenboom 1, C. van Weelden 1, C.B.M. Blom 1, 1 Delft University of Technology, the Netherlands Gemeentewerken Rotterdam, the Netherlands In
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationWave propagation in a magnetoelectroelastic
Science in China Series G: Physics Mechanics & Astronomy 008 SCIENCE IN CHINA PRESS SpringerVerlag www.scichina.com phys.scichina.com www.springerlink.com Wave propagation in a magnetoelectroelastic
More informationC:\Users\whit\Desktop\Active\304_2012_ver_2\_Notes\4_Torsion\1_torsion.docx 6
C:\Users\whit\Desktop\Active\304_2012_ver_2\_Notes\4_Torsion\1_torsion.doc 6 p. 1 of Torsion of circular bar The crosssections rotate without deformation. The deformation that does occur results from
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationHomework of chapter (1) (Solution)
بسم اهلل الرمحن الرحيم The Islamic University of Gaza, Civil Engineering Department, Fluid mechanicsdiscussion, Instructor: Dr. Khalil M. Al Astal T.A: Eng. Mohammed H El Nazli Eng. Sarah R Rostom First
More informationAXISYMMETRIC ELASTICITY PROBLEM OF CUBIC QUASICRYSTAL *
Volume 9, Number April, 9963//9/9 CHINESE PHYSICS c Chin. Phys. Soc. AXISYMMETRIC ELASTICITY PROBLEM OF CUBIC QUASICRYSTAL * Zhou Wangmin and Fan Tianyou Research Center of Materials Science, Beijing
More informationA Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials
Dublin, October 2010 A Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials FracMan Technology Group Dr Mark Cottrell Presentation Outline Some Physical
More information